HydrogenStorage web.mit.edu/dincalab/papers/ opposed to stationary storage, in which the tank volume
Embed Size (px)
Transcript of HydrogenStorage web.mit.edu/dincalab/papers/ opposed to stationary storage, in which the tank volume
Hydrogen Storage DOI: 10.1002/anie.200801163
Hydrogen Storage in Microporous Metal–Organic Frameworks with Exposed Metal Sites Mircea Dincă and Jeffrey R. Long*
Keywords: bond dissociation energy · hydrogen storage · metal– H2 binding · metal– organic frameworks · microporous materials
J. R. Long and M. DincăReviews
6766 www.angewandte.org � 2008 Wiley-VCH Verlag GmbH & Co. KGaA, Weinheim Angew. Chem. Int. Ed. 2008, 47, 6766 – 6779
Hydrogen is one of the leading candidates as an energy carrier of the future because of its high energy content and clean burning, potentially renewable nature. A particularly daunting challenge facing its use in transportation, however, is the development of a safe and practical storage system. As opposed to stationary storage, in which the tank volume and mass are less of a concern, storage of large quantities of H2 in a passenger car, for which volume, mass, and heat exchange are of utmost importance, presents a formidable scientific and engineering endeavor. Many reports have dealt with the use of hydrogen as a fuel and its storage in different solid-state media and in high-pressure or cryogenic tanks. Among the newer materials, crystalline microporous solids comprised of metal building units and organic bridging ligands, known as metal–organic frameworks (MOFs), are perhaps the most promising physisorption candidates. However, because of their typically weak interaction with H2, dominated by dispersion forces, these materials function best only at very low temperature and their use as storage media in vehicles would require cryogenic cooling.
To eliminate the need for a heavy and expensive cooling system, new ways of increasing the hydrogen affinity of these materials must be devised. In some cases, this has been achieved by minimizing the size of the pores, which enhances the van der Waals contacts with the H2 molecules,
 or by sequestering hydrogen inside flexible metal–organic frame- works, which then show hysteretic adsorption behavior and are able to desorb hydrogen at increased temperature.
Additionally, several reports have shown that coordinatively unsaturated metal centers embedded within metal–organic frameworks can participate directly in the binding of H2, resulting in some of the highest binding energies reported thus far for high-capacity microporous materials. Given that metal–organic frameworks can be tailored to incorporate a large number of selected metal cations, this method presents a promising strategy for achieving the H2 binding energy required for storage near room temperature.
2. Hydrogen Storage Requirements
2.1. The US DoE Storage System Targets
Recent research on hydrogen storage has been guided by the requirements set forth by the United States Department of Energy in 2003 and amended in 2006. These targets were set under the assumption that future hydrogen-fueled cars should have a range of 300 miles (480 km), should operate under ambient conditions, and should allow fast, safe, and efficient fueling, similar to gasoline. Ultimately, safety con- cerns will limit the maximum allowed pressure for a storage device to 100 bar, meaning that solid-state materials that can be cycled at lower pressures than compressed-gas cylinders must be developed.
Because hydrogen contains three times the energy of gasoline per unit mass, it was estimated that a hydrogen storage tank would have to carry approximately 5 kg of H2. As such, the 2010 DoE capacity targets for a fueling system (including the tank and its accessories) have been set at 6 wt% and 45 gL�1 of usable H2. The targets also specify that the system should show no decay for 1000 consecutive fueling cycles and should allow filling to full capacity in less than 3 min. The 2015 system targets are even more demanding: 9 wt% and 60 gL�1 of H2, 1500 cycles, and a fueling time of 2.5 min. If achieved together, these targets would lead to the same efficiency as current gasoline tanks. The immense difficulty of accomplishing the above targets becomes clear, however, when one notes that 5 kg of hydrogen occupies a volume of 56000 L under ambient conditions, and that 5 kg of liquid hydrogen would still require a 70 L cryogenic tank.
Owing to their high uptake capacity at low temperature and excellent reversibility kinetics, metal–organic frameworks have attracted considerable attention as potential solid-state hydrogen storage mate- rials. In the last few years, researchers have also identified several strategies for increasing the affinity of these materials towards hydrogen, among which the binding of H2 to unsaturated metal centers is one of the most promising. Herein, we review the synthetic approaches employed thus far for producing frameworks with exposed metal sites, and summarize the hydrogen uptake capacities and binding energies in these materials. In addition, results from experi- ments that were used to probe independently the metal–hydrogen interaction in selected materials will be discussed.
From the Contents
1. Introduction 6767
2. Hydrogen Storage Requirements 6767
3. H2 Binding to Metal Species 6768
4. Metal–Hydrogen Binding in Metal–Organic Frameworks 6771
5. Strategies for Incorporating Unsaturated Metal Centers in Metal–Organic Frameworks 6774
6. Conclusion and Outlook 6777
[*] M. Dincă, J. R. Long Department of Chemistry University of California, Berkeley Berkeley, CA 94720-1460 (USA) Fax: (+1) 510-643-3546 E-mail: email@example.com Homepage: http://alchemy.cchem.berkeley.edu
Hydrogen Storage Angewandte
6767Angew. Chem. Int. Ed. 2008, 47, 6766 – 6779 � 2008 Wiley-VCH Verlag GmbH & Co. KGaA, Weinheim
Moreover, both of these calculations ignore the mass and volume of the container and of the cooling system.
2.2. Adsorption Enthalpy Requirements for Physisorptive H2 Storage
Clearly, significant innovations are necessary to build a viable hydrogen storage system. As stated before, the greatest challenge for physisorptive materials is to increase the strength of the H2 binding interaction. Recently, Bhatia and Myers addressed this issue by employing the Langmuir equation to derive relationships between the operating pressures of a storage tank and the enthalpy of adsorption required for storage near room temperature. Using P1 and P2 as the lower and upper bounds of the operating pressure and approximating the H2 adsorption entropy as DS
(R = ideal gas constant), they derived Equation (1). They then used this equation to show that a microporous material operating between 1.5 and 30 bar at 298 K should have an average optimal adsorption enthalpy DH�opt of 15.1 kJmol
�1. Similarly, if P2 is increased to 100 bar, the required average adsorption enthalpy decreases to 13.6 kJmol�1.
DH�opt ¼ T DS�optþ R T 2
P1 P2 P20
In the same work, Bhatia and Myers derived Equation (2), which can be used to calculate the optimal operating temper- ature Topt of a hydrogen storage material for a given average enthalpy of adsorption DH�ads. This relationship can be used to show that a microporous material with DH�ads = 6 kJmol
�1, which is a typical value for current metal–organic frameworks
and other microporous solids, can operate between 1.5 and 100 bar at an optimal temperature of 131 K.
Topt ¼ DH�ads
½DS�adsþ ðR=2ÞlnðP1 P2=P20Þ ð2Þ
3. H2 Binding to Metal Species
As the simplest known chemical compound, the hydrogen molecule has been the subject of countless experiments and theoretical investigations, leading to some of the most fundamental discoveries in the areas of electronic structure and chemical bonding. Although metal complexes with other relatively unreactive small molecules, such as N2, H2C=CH2, and even CO2, had been known for many years,
 the first metal complex of an H2 molecule was not isolated until 1984, when Kubas and co-workers reported the now famous “Kubas complex” [W(CO)3(PiPr3)(H2)] (iPr= isopropyl).
 Using single-crystal neutron diffraction and a variety of other techniques, they later showed that this complex contained a side-on bound H2 ligand with an H�H distance only slightly elongated relative to that in gaseous H2, thus unequivocally proving that the complex was not a classical dihydride.
Subsequent to this seminal discovery, s-H2 complexes of virtually every transition metal have been reported, and their properties and reactivity have been the subject of many excellent review articles and a comprehensive book by Kubas.
Surprisingly, despite the large number of s-H2 complexes that have been reported so far, the vast literature on the subject contains very few studies that address the thermody- namic properties of the metal–H2 interaction, and in partic- ular the bond dissociation energy (BDE) of the metal–H2 bond. Vibrational spectroscopy, variable-temperature NMR spectroscopy, or photoacoustic calorimetry have been used to quantify this interaction in only a handful of organometallic complexes (Table 1). The BDE values obtained for many of these complexes are affected by the fleeting formation of solvento species or by the presence of agostic C–H inter- actions. For example, formation of the transient complex [(C6H5Me)Cr(CO)2(Xe)] allowed only an approximate mea- surement of the energy of dissociation of H2 from [(C6H5Me)Cr(CO)2(H2)], which was estimated at 70 kJmol�1. The energy of the agostic C–H interaction, which affects particul